glassy polymers. 4. comparison of five 4 (1).pdf rate," vapor-induced swelling ......
Post on 27-Sep-2018
Embed Size (px)
Reprinted from Macromolecules, 1983. 16, 898 Copyright g 1983 by the American Chemical Society and reprinted by permission of the copyright owner.
Effects of Annealing and Prior History on Enthalpy Relaxation in Glassy Polymers. 4. Comparison of Five Polymers
Ian M. Hodge
BFGoodrich Research and Development Center, Brecksville, Ohio 44141. Received October 27, 1982
ABSTRACT: Parameters for enthalpy relaxation in and below the glass transition temperature range were determined for poly(vinyl acetate) (PVAc), poly(methyl methacrylate) (PMMA), and bisphenol A polycarbonate (PCarb) and compared with those previously obtained for another PVAc, two polystyrenes (PS), poly(vinyl chloride) (PVC), the inorganic glasses As 2Se3 and B203 , and the simple organic glass 5-phenyl 2-ether. The four-parameter treatment of Moynihan and co-workers was found to give an adequate description of the relaxation component of the heat capacity, as a function of cooling rate, annealing temperature, and annealing time, for PVAc and PCarb. Significant deviations were found for PMMA. Strong correlations were observed between all four parameters for the five polymers, which were interpreted in terms of a cooperative relaxation mechanism.
Introduction Annealing of amorphous polymers below the glass
transition temperature range produces changes in many physical properties such as density, complex permittivity, enthalpy, complex mechanical modulus, and creep com-pliance. A particularly convenient property for the study of annealing is enthalpy, because of the availability of accurate and sensitive DSC instruments. The decrease in enthalpy during annealing is recovered during reheating to above the glass transition, and this recovery is usually manifested as a maximum in the heat capacity at tem-peratures ranging from well below to near the upper edge of the glass transition range. Recovery of the enthalpy lost during annealing has been observed in many polymeric materials, 1 '8 and a sufficiently large amount of experi-mental data has now been collected to permit several generalizations to be made:
(1) The temperatures, Tmax , at which the heat capacity maxima, Cp.., occur increase approximately linearly with annealing temperature, Te , and the log of the annealing time, t e, provided the aged glass is not too close to equi-librium. Also, T approximately linearly with the log of the heating rate, QH. It also appears that T is insensitive to the history before aging, such as cooling rate," vapor-induced swelling,' hydrostatic pressure ap-plied during cooling,5,9,11,15 or mechanical straining. 6,16,18
(2) The magnitude of Cp... also increases approximately linearly with Te and log te, again providing that the aged glass is not too close to equilibrium. In contrast to T , however, Cp.. is a strong function of prior history. Gen-erally speaking, those histories that elevate the enthalpy of the glass before annealing serve to increase C Similar Aug' behavior is observed for the enthalpy lost during aging, AH, of which Cp is a crude measure.
(3) As the agedrglass approaches equilibrium deviations from these linear relations are observed, until at equilib-rium no changes occur with annealing. At fixed t e, AH and Cp.. pass through maxima as a function of Te , often when Te is about 20 K below the center of the glass transition range, Tg, and decreases to zero when Te is well above Tg. At fixed Te , AH becomes constant at long t e as the aged glass approaches equilibrium.
The first reported observations of heat capacity maxima well below Tg in aged glasses appear to be those of niers.' The first theoretical account of this phenomenon was that of Kovacs et al.," given in terms of a multiparameter model for the glass transition which included the well-established nonlinearity and nonexponentiality (relaxation time dis-tribution) of the glass transition kinetics. Recently Hodge and Berens2 gave a physically similar, but mathematically
different, account in terms of the four-parameter treatment of the glass transition kinetics by Moynihan and co-workers" and demonstrated explicitly that all of the general features listed above could be reproduced by this approach. Good fits to data for poly(vinyl chloride , (PVC) were also obtained for several combinations of Te and t e. Hodge and Huvard22 demonstrated that the four param-eters of the Moynihan formulation could be optim ized by using a standard computer search routine, and applied this optimization procedure to data for two polystyrenes (PS). For the present work essentially the same technique was applied to data for poly(vinyl acetate) (PVAc), poly (methyl methacrylate) (PMMA), and bisphenol A polycarbonate (PCarb). The enthalpy relaxation parameters for these materials were compared with those already found for PVC,2 PS,22 another PVAc:," B203," As2Se3 ,24 and the lubricating oil C 6H5(0C6H4)30C6H5 ("5-phenyl 4-ether" or "5P4E") 24 by using the same formalism.
For convenience we outline the treatment of the glass transition kinetics of Moynihan arid co-workers, 21 how annealing was introduced by Hodge and Berens, 2 and the optimization procedure used by Hodge and Huvarci. 22 The glass transition kinetics are characterized by two essential featuresnonexponentiality (relaxation time distribution) and nonlinearity. The Moynihan approach linearizes the kinetics by using the method of Gardon and Narayana-swamy,25,26 considers cooling and heating as a series of temperature steps, and applies Boltzmann superposition of nonexponential responses to the temperature steps. As a matter of convenience, and good accuracy, the response function is chosen to be of the Williams-Watts 2' ,29 form
Oft) = exP[-- (t/Tor] (1)
where 1 > 0 and To is a relaxation time which depends on temperature, T, and fictive temperature, 29 Tf, as
thh* (1 _ x)Ah* To = A exp
RT RTf (2)
where A, x (1 x > 0), and Ah* are parameters and R is the ideal gas constant. The four parameters 0, A, x, and Ah* are assumed to be independent of T and T. Hodge and Berens 2 introduced annealing into the cooling cycle, with the annealing time divided into ten logarithmically even spaced subintervals to allow for nonlinearity during annealing. Hodge and Huvard 22 used an optimization technique based on the Marquardt search routine- 30 The thermal history (cooling rate, annealing temperaimre, an-nealing time, and reheating rate) and Ah* were input, and the best fit values of A, x, and 0 were output. The best-fit
Macromolecules, Vol. 16, No. 6, 1983
Table I Polymer Molecular Weights
material Mw Mr, MW /ME ref
PVAc -1.95 x 10 4.77 X 104 4.1 this work PVAc 2.0 x 106 3.4 x 10' 5.9 23 PVC 2.05 x 10 5 6.5 x 104 3.2 18 PS 3.21 x 10' 8.46 x 10 4 3.8 22 PS 2 x 10' 2 x 10'
2.2- te 1 Hour - Te = 300K
- 40 /+ 10
01 1 o i o e
1 1 300 310 320 330
1/K Figure 2. Experimental points and fits for CpN for the indicated combinations of T0 and te for PVAc. Parameters same as in Figure I.
1 foV=9--0 _
_ 51+10 f 101+10 p 1 f _ I
- I I- oi - ....eled - c3-0
I 1 i I I I I I I 1 360 370 380 390 400 360 370 380 390 400
T/K T/ K
Figure 3. Experimental points and fits for C pN as a function of cooling rate for PMMA. Best fit parameters given in Table II.
Table II. These parameters were all obtained by using the Moynihan formulation, and are thus directly compa-rable.
The fits for PVAc (Figures 1 and 2) and PCarb (Figures 5 and 6) deviate from the data by less than the experi-mental uncertainty, indicating that the model provides an adequate account of enthalpy relaxation in these materials. The fits to PMMA deviate from the experimental data by
Macromolecules, Vol. 16, No. 6, 1983
70 = 350 1.0 te I Hour
_ T. = 360
te = I Hour
,o/.7cP _ 0
360 370 380 390 400
Figure 4. Experimental points and fits for CpN for the indicated combinations of T. and t. for PMMA. Parameters same as in Figure 3.
- - A Cp
N 5 / + 10 L. 10/4-10 Ti _ _
/ . _ .6....1) _ 0 _ . _ ...I
T/K T/K _
P ) -
1.0 201+10 401+10 flLoo p ea0 ..0..0..
N - 6 - 1 Cp _
/ - i
- o -
- ..0.....61 - 0 - - 400 410 420 430 440 400 410 420 430 440
T / K T/K
Figure 5. Experimental points and fits for C pN as a function of cooling rate for PCarb. Best fit parameters given in Table II.
up to 17%, well outside experimental uncertainty, although the occurrence of sub- Tg shoulders and maxima in CpN in annealed glasses is qualitatively reproduced. Evidently there is at least one feature of the enthalpy relaxation kinetics for PMMA that is not being properly accounted for in the model. Accordingly, the uncertainties in the enthalpy relaxation parameters for PMMA are larger than those for the other materials (see Table II).
The parameters obtained for PVAc agree within un-certainty limits with those obtained by Sasabe and Moy-nihan,23 except for x, where the difference is slightly greater than the sum of uncertainties. The similarity of the en-thalpy relaxation parameters for these two PVAc materials
Macromolecules, Vol. 16, No. 6, 1983
Enthalpy Relaxation in Glassy Polymers 901
T8 = 390 I Wells,
te = 16 Hours
5P4E o PVAc (Ref. 23) 0 PVC (Ref. 18)
- 4 A PVA